JOURNAL OF APPLIED PHYSICS 106, 073504 共2009兲

Strain-induced variations of electronic energy band edges of embedded semiconductor quantum dots in half-space substrates Ernie Pan,1,a兲 Yu Zou,1 Peter W. Chung,2 and John D. Albrecht3 1

Computer Modeling and Simulation Group, College of Engineering, University of Akron, Akron, Ohio 44325, USA 2 U.S. Army Research Laboratory, Aberdeen Proving Ground, Maryland 21005, USA 3 Air Force Research Laboratory, WPAFB, Ohio 45433, USA

共Received 15 July 2009; accepted 24 August 2009; published online 7 October 2009兲 The strain-induced local electronic band edge states in semiconductor quantum dots 共QDs兲 are studied using a k · p description of the electronic eigenstates coupled with the induced lattice strain as calculated using the continuum mechanics 共CM兲 description. In the CM method, the misfit-lattice induced strain can be reduced to an analytical expression that is straightforward to evaluate numerically. Different from most previous analyses for QDs in infinite spaces, we address cubic and pyramidal QDs located in half-space substrates with different lattice orientations, which more realistically describe experimental situations in most instances. The band edges within the cubic and pyramidal InAs QDs embedded in GaAs substrates are predicted within the six-band k · p basis via both a published approximation and the presented exact approach. Comparison of the strain-induced local band edge shows that the approximate method adopted previously in literature could result in a substantial error near the interface region of the QD. The strain-induced band edges along the bottom center line of the QD can differ by a factor of 2 between the two approaches. Furthermore, the effect of the free surface on the strain-induced band edges is studied by varying the depth of the buried QD. When the QD is moved away from the surface, the band edges converge in a consistent way to the infinite-space solution. Comparison with available experimental results validates our exact model within the half-space substrate and shows the importance of treating the surface in a theoretically rigorous way. © 2009 American Institute of Physics. 关doi:10.1063/1.3234383兴 I. INTRODUCTION

Quantum-dot 共QD兲 heterostructures have been increasingly sought for applications as novel materials and devices such as gain media for semiconductor lasers. Their unique properties arise from quantum confinement and are known to be further sensitive to strain-perturbed fields that modify the electronic states, and subsequently the optoelectronic properties.1–3 Strain is increasingly a useful variable with which bandgap energies, and subsequently exciton energies, can be designed into devices.4 The sensitivity of the bands to strains can be substantial. The strain-induced level shifts in the bandgap of InAs/GaAs QDs in some cases may approach the gap sizes of the semiconductor.5 There are a couple of theoretical/numerical studies on the effect of strain on the band edges in pyramidal QDs. For example, an original technique based on a plane-wave expansion method to calculate the electron and hole wave spectra was presented by Andreev and O’Reilly,6 including the three-dimensional strain and built-in electric field distributions. Ranjan et al.7 studied the optical properties of strained GaN QDs using a tight-binding method. Grundmann et al.8 simulated numerically a pyramidal QD on a thin wetting layer using the finite difference method and also calculated the corresponding electronic structure and the opticalphonon energies. The strain distribution of self-assembled pyramidal InGaAs/GaAs QDs and the dependence of the biaxial and hydrostatic components on the QD volume, aspect a兲

Electronic mail: pan2@uakron.edu.

0021-8979/2009/106共7兲/073504/12/$25.00

ratio, and composition were calculated by Califano and Harrison9 using Green’s function-based technique. With refined meshes and grids, these numerical methods can predict very good strain profiles and confining potentials. In general, the theories/models for analyzing the misfitlattice induced strain field and the corresponding band structure in low-dimensional QD systems can be categorized as the continuum mechanics 共CM兲 based method10–13 and the valence force field14,15 method for the calculation of the strain field, and the empirical tight-binding model,16–18 empirical pseudopotential model,19,20 and the k · p model21 for the calculation of the band structure. However, we point out that in most of the previous research, the QD was assumed to be in an infinite-space material matrix or substrate. Furthermore, in applying the six-band k · p model for bandgap edge calculation, the induced shear strain and the normal strain difference were both neglected. In this paper, we assume that the QD is buried within a half-space substrate where the distance from the QD to the surface is arbitrary. As such, the induced strain field and the local band edge will be influenced by the existence of a free boundary, resulting in different strain and band edge features as compared to those in an infinite space. Further, to calculate the elastic field induced by the QD, the analytical Green’s function method presented by Pan et al.22 is employed, where the QD surface is approximated by a number of flat triangles so that the required boundary integration can be carried out exactly. Based on our analytical solution for the induced strain field, we predict the strain-related local band edge for the InAs QD within the GaAs substrate using

106, 073504-1

© 2009 American Institute of Physics

073504-2

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

shear strain and the strain difference between ␥xx and ␥yy.15,31,32 By doing so, one is able to derive simple closedform expressions for the electronic states at the conduction band 共CB兲 and valence band 共VB兲 edges and evaluate the relative significance of different treatments of the lattice strain. It is apparent that this approximation would be acceptable if the shear strain is very small and the deformation is such that ␥xx = ␥yy. In general, however, one should be cautious in making such an assumption, as will be illustrated later with numerical examples. We limit our consideration to the local band edges 共at k = 0兲 pertinent to many of the direct bandgap semiconductor QD systems of this class. At the zone center the CB and VB models can be decoupled and the latter can be further characterized by a six-band Hamiltonian. We adopt the accepted standard notation for wave function basis functions as follows:33

the six-band k · p model 共for both the exact and approximate approaches兲. Our numerical results show that the free surface of the substrate could have a significant influence on the bandgap edge and that the exact k · p model has to be employed in the strain-induced bandgap prediction. This conclusion is further confirmed by previous experimental results against which the approximate six-band k · p model shows a large error in the band edge calculation. This paper is organized as follows: Green’s function method for calculating the misfit-lattice induced elastic strain and the analytical multiband k · p model for evaluating the strain-induced band edge shifts are introduced in Sec. II. Numerical results for cubic and pyramidal InAs QDs within GaAs 共001兲 and 共111兲 substrates are presented in Sec. III, along with a comparison to published experimental data for validation. Conclusions are drawn in Sec. IV.

兩 23 , 23 典 = − 冑12 兩共x + iy兲↑典,

II. MISFIT-LATTICE INDUCED ELASTIC STRAIN FIELD AND K · P MODEL FOR ZINCBLENDE QD

兩 23 , 21 典 = 冑16 兩− 共x + iy兲↓+ 2z↑典,

To simplify the strain calculation, we adopt the Eshelby inclusion approach, which assumes that the material properties between the QD and the substrate are the same.6,23 By doing so, the induced elastic strain can be obtained by simple integration of the analytic Green’s functions over the QD surface.22 Furthermore, for the QD made of piecewise flat surfaces, the involved surface integration can be exactly carried out. Therefore, the QD-induced elastic strain can be accurately predicted based on our Green’s function method.22,24–27 We point out that although the complex inhomogeneity model was proposed to study the strained quantum structure,28 finding reliable material properties in the QD and quantum wire is still a challenge.29 In order to calculate the band edges, we use the established multiband k · p method that accounts for the strain effects with related parameters being determined empirically and/or experimentally.30 Without sacrificing the salient physical characteristics for this investigation, the Hamiltonian matrix could be further simplified by suppressing the

H=−

冢

− S␥

R␥

0

−

− S ␥+

P␥ − Q␥

0

R␥

− 冑2Q␥

R ␥+

0

P␥ − Q␥

S␥

0

R ␥+

S ␥+

−

1

冑2 S ␥

冑2R␥+

+

− 冑2Q␥

冑

3 + S 2 ␥

冑

3 S␥ 2

冑2Q␥

兩 23 ,− 23 典 = 冑12 兩共x − iy兲↓典, 兩 21 , 21 典 = 冑13 兩共x + iy兲↓+ z↑典, 兩 21 ,− 21 典 = 冑13 兩共x − iy兲↑− z↓典,

冑2R␥

冑

−

1

冑2

S␥

3 S␥ 2

冑2Q␥

3 + S 2 ␥

P␥ + Q␥ − 冑2R␥+ − − 冑2R␥

共1兲

where 兩x典, 兩y典, and 兩z典 indicate the symmetry of the VB zone center states, and ↓ and ↑ denote the spin orientations. According to the theory of Luttinger and Kohn,34 and Bir and Pikus,35 the VB band structure 共at k = 0兲 of a strained bulk semiconductor can be described by the following 6 ⫻ 6 Hamiltonian in the envelope-function space 关including the heavy hole 共HH兲 共兩3 / 2 , ⫾ 3 / 2典兲, light hole 共LH兲 共兩3 / 2 , ⫾ 1 / 2典兲, and spin-orbit split-off bands 共SO兲 共兩1 / 2 , ⫾ 1 / 2典兲兴:

1

冑2 S ␥

P␥ + Q␥

冑

兩 23 ,− 21 典 = 冑16 兩共x − iy兲↑+ 2z↓典,

1

冑2

S ␥+

P␥ + ⌬

0

0

P␥ + ⌬

冣

冏 冏 冏 冏 冏 冏

3 3 , 2 2 3 1 , 2 2

冔 冔 冔 冔 冔 冔

3 1 ,− 2 2 3 3 ,− 2 2 1 1 , 2 2

1 1 ,− 2 2

,

共2兲

073504-3

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

where ⌬ is the spin-orbit split-off energy and “+” denotes the Hermitian conjugate of the matrix elements. The key straindependent elements in the matrix are defined as P ␥ = − a v␥ H ,

共3a兲

b Q␥ = − ␥B , 2

共3b兲

R␥ =

冑3 2 b共␥xx

− ␥yy兲 − id␥xy ,

S␥ = − d共␥xz − i␥yz兲,

共3c兲 共3d兲

where ac, av, b, and d are the Pikus-Bir deformation potential constants for the CB and VB; and ␥H = ␥xx + ␥yy + ␥zz and ␥B = ␥xx + ␥yy − 2␥zz are defined as the hydrostatic and biaxial strains, respectively. We will focus our attention on the local band edge modification based on the induced strain, as in Pryor’s paper.36 That is, we will calculate the eigenvalues of strain-dependent Hamiltonian 共2兲. In general, the eigenvalues of Eq. 共2兲 need to be solved numerically. However, if one further assumes that S␥ = R␥ = 0, i.e., ignoring the shear strain and the normal strain difference between ␥xx and ␥yy, then the eigenvalues of matrix 共2兲, as the strain-induced band edge shifts of VB, can be obtained analytically as b EHH = − P␥ − Q␥ = av␥H + ␥B , 2

共4a兲

1 ELH = − P␥ + 共Q␥ − ⌬ + 冑⌬2 + 2⌬Q␥ + 9Q␥2兲 = av␥H 2 1 1 b − ␥B − ⌬ + 2 2 4

冑

9 ⌬2 − ⌬b␥B + b2␥B2 , 4

共4b兲

1 ESO = − P␥ + 共Q␥ − ⌬ − 冑⌬2 + 2⌬Q␥ + 9Q␥2兲 = av␥H 2 1 1 b − ␥B − ⌬ − 2 2 4

冑

9 ⌬2 − ⌬b␥B + b2␥B2 . 4

共4c兲

On the other hand, by assuming the unstrained bandgap as Eg0, the relative CB edge energy is given by EC = Eg0 + ac␥H .

共5兲

III. NUMERICAL RESULTS AND COMPARISON TO EXPERIMENTS

In this section, cubic and pyramidal InAs QDs in 共001兲 and 共111兲 GaAs half-space substrates are investigated兲. The ⴱ misfit-lattice eigenstrain in the QD is hydrostatic, i.e., ␥xx ⴱ ⴱ = ␥yy = ␥zz = 0.07. The origin 共0,0,0兲 of the coordinate system is on the surface of the half plane, and the z-axis points down vertically. Both cubic and pyramidal QDs have the same height 共h = 4 nm兲, same volume, and the same vertical distance to the surface 共d = 4 nm兲 from their middle plane but with different base lengths 共b = 8.62 nm for cubic and b = 14.93 nm for pyramidal QD兲. Other involved material

FIG. 1. Schematic of InAs QDs in GaAs substrates: cubic QD in 共a兲 and pyramid QD in 共b兲. Both QDs have the same distance between the body center and the surface of half plane: d = 4 nm; strain and band edge results are along the dashed-dotted lines and the z-axis.

properties and parameters are listed in the Appendix. Numerical results are presented via both approximate method 共4兲 where the shear strain and the normal strain difference between ␥xx and ␥yy are neglected and the exact method where the eigenenergies of Hamiltonian 共2兲 are solved directly without the above approximation. The results for the strain-induced CB edge based on Eq. 共5兲 are also shown in the figures. Furthermore, comparison with the available experimental results validates our exact model within the halfspace substrate, and thus demonstrates that the influence of the surface is important and that the approximate approach for band edge calculation is not valid near the boundary of the QDs. We point out that in the 共111兲-direction case, there will be an induced piezoelectric field. However, this induced piezoelectric field has a negligible effect on the bandgap within the QD for group III-V semiconductors since the piezoelectric couplings in these materials are very weak.37,38 Its influence outside the QD could be important 共e.g., lowers the symmetry of the involved system, leads to a lifting of degeneracy, etc兲.8 This will be addressed in the future using the fully coupled piezoelectric model, which can be applied to the strongly coupled III nitrides as well as the weakly coupled group III-V semiconductors.38

A. Local band edges in a cubic InAs QD embedded in „001… and „111… GaAs half-space substrates

The local band edge energies within the embedded InAs QD along three dashed-dotted lines 关see Fig. 1共a兲兴 are investigated via both the exact and approximate methods. The first line is on the bottom plane of the cubic QD at fixed y = 0 nm and z = 6 nm, with x varying from ⫺3.71 to 3.71 nm. The second line is along the z-axis, i.e., at fixed y = 0 nm and x = 0 nm, with z varying from 2 to 6 nm. The third line is along a specific vertical line where x and y are fixed at 2.15 and 0 nm, with z varying from 2 to 6 nm. All these lines are within the QD so that we can systematically study the features of cubic QD band edges in a half-space. The strain components and band edge values along the first dashed-dotted line are shown in Figs. 2共a兲–2共d兲 for a cubic QD in GaAs 共001兲 and GaAs 共111兲 substrates. As shown in Figs. 2共a兲 and 2共c兲, the biaxial strain ␥B is always positive within the QD domain thus inducing a higher energy level in LH band than in HH band, which is consistent with previous work.32,36,39 The strain components R␥ and S␥ 关expressed by Figs. 2共c兲 and 2共d兲兴, which represent the contributions from the shear strain and the normal strain difference

073504-4

Pan et al.

J. Appl. Phys. 106, 073504 共2009兲

FIG. 2. 共Color online兲 Strain components 关共a兲 and 共c兲兴 and band edges 关共b兲 and 共d兲兴 in a cubic InAs/GaAs QD along the bottom center line of the QD 关共a兲 and 共b兲兴 in 共001兲 substrate and 关共c兲 and 共d兲兴 in 共111兲 substrate.

between ␥xx and ␥yy, clearly indicate that their magnitude increases from the center to the lateral boundary of the QD. Consequently, one would expect that the band edge based on the exact and approximate methods could be different, particularly near the lateral boundary area of the QD. It is also apparent from Figs. 2共b兲 and 2共d兲 that the band edge difference between the two methods is larger in the InAs QD embedded in GaAs 共111兲 than that in GaAs 共001兲. Along the second dashed-dotted line, the shear strain and normal strain difference between ␥xx and ␥yy are close to zero due to the symmetry of the geometry about the z-axis 关R␥ and S␥ shown in Figs. 3共a兲 and 3共c兲兴. Therefore, the band edges based on the two methods are nearly identical, even near the boundary of the QD 关Figs. 3共b兲 and 3共d兲兴. Along the third line, which is an off-center vertical line, R␥ and S␥ are not zero, particularly near the boundary of the QD as in Figs. 4共a兲 and 4共c兲. Therefore, some differences in the band edges based on the two methods are observed near the boundary, as shown in Figs. 4共b兲 and 4共d兲. Again the difference is larger in GaAs 共111兲 than in GaAs 共001兲.

B. Local band edges in a pyramidal InAs QD embedded in „001… and „111… GaAs half-space substrates

The numerical results for the strain components and local band edges in pyramidal InAs QD embedded in GaAs 共001兲 and GaAs 共111兲 are shown in Figs. 5–7. Figure 5 shows the result along the first dashed-dotted line, i.e., the center line on the bottom of the QD 共for y = 0 nm and z = 6 nm, with x varying from ⫺7.464 to 7.464 nm兲. It is obvious that the results are symmetric 共on the positive and negative x sides兲 for the QD in GaAs 共001兲 but is slightly asymmetric in GaAs 共111兲, particularly for the shear strain component 关Fig. 5共c兲兴. Similar to the cubic QD, we observe apparent differences between the approximate and exact methods near the lateral boundary of the QD. Figure 6 shows the strain components and local band edges along the second dashed-dotted line, i.e., for x = y = 0 nm with z varying from 2 to 6 nm, within the InAs QD based on both methods. It is clear from Figs. 6共a兲 and 6共c兲 that the strain distribution in a pyramidal QD is quite differ-

073504-5

Pan et al.

J. Appl. Phys. 106, 073504 共2009兲

FIG. 3. 共Color online兲 Strain components 关共a兲 and 共c兲兴 and band edges 关共b兲 and 共d兲兴 in a cubic InAs/GaAs QD along the z-axis of the QD 关共a兲 and 共b兲兴 in 共001兲 substrate and 关共c兲 and 共d兲兴 in 共111兲 substrate.

ent than that in a cubic QD along this line. For instance, the ␥H has a relatively large change, which induces a large drop in the CB curve near the apex of the pyramid. Furthermore, the energy level of the LH is always higher than that of the HH because of the positive value of ␥B as in cubic QD 关Figs. 3共b兲 and 3共d兲兴. Finally, Fig. 7 shows the band edge within the pyramidal QD along the third dashed-dotted line, i.e., along the special vertical line at x = 4.33 nm and y = 0 nm with z varying from 4.32 to 6 nm. Compared to the other two lines, the studied points are closer to the QD boundary, and thus an apparent difference in the band edge between the approximate and exact methods exists along the entire line, as shown in Figs. 7共b兲 and 7共d兲. As in the cubic QD case, the band edge discrepancy in the QD embedded in GaAs 共111兲 is larger than that embedded in GaAs 共001兲. In summary, there are some interesting features in the QD-induced strain and band edge distributions within the InAs QD embedded in the GaAs 共001兲 and GaAs 共111兲 halfspace substrates: First, the ␥H shifts both the CB and VB edges, and both the ␥B and ⌬ contribute to the splitting between HH and LH while the ⌬ only introduces the splitting

between LH and SO band edges. Second, the band edge of LH is always higher than that of HH because of the positive ␥B. Third, in some cases, large differences in band edges based on the exact and approximate methods may exist in the QD domain, as is further discussed in Sec. III C. C. Band edge error based on the approximate method

The approximate and exact methods were compared for band edge values at specific locations as depicted in Fig. 1. Among the three lines—one parallel and two perpendicular to the surface of the substrate—the difference between the two calculation methods is the largest for points in the line parallel to the surface. The difference between the two methods is always large near the boundary of the QD. Also, we can see clearly, from Fig. 2 to Fig. 7, that the band edge difference in QDs embedded in the 共111兲-oriented GaAs substrate is larger than that in QDs embedded in the 共001兲oriented substrate. Here we further study the error in the strain-induced local band edge based on the approximate method where the

073504-6

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

FIG. 4. 共Color online兲 Strain components 关共a兲 and 共c兲兴 and band edges 关共b兲 and 共d兲兴 in a cubic InAs/GaAs QD along the specified vertical line of the QD 关共a兲 and 共b兲兴 in 共001兲 substrate and 关共c兲 and 共d兲兴 in 共111兲 substrate.

shear strain and the normal strain difference between ␥xx and ␥yy are neglected. We define the relative error as

error共%兲 =

兩Ei − eig共H兲兩 ⫻ 100%, 兩eig共H兲兩

the bottom center line, one has to use the exact eigenvalue solution method to predict the strain field and its induced local band edges.

共6兲

where Ei refers to the energies calculated from Eqs. 共4a兲–共4c兲 using the approximate method, and eig共H兲 refers to the eigenvalues of Hamiltonian matrix 共2兲 using the exact method. The relative errors are shown in Figs. 8共a兲 and 8共b兲 for points along the bottom center line and along the z-axis, respectively, for cubic InAs QD embedded in GaAs half-space substrates with 共001兲 and 共111兲 orientations. It is observed that along the z-axis, the relative error is very small 共the biggest error is around 1%兲 关Fig. 8共b兲兴; while along the bottom center line of the QD, the relative error can be as large as 100% 关Fig. 8共a兲 near the lateral boundary of the QD兴. We also note that the error curves for a QD in the GaAs 共111兲 substrate are asymmetric because of the asymmetric strain and energy distribution 关as shown in Figs. 2共c兲 and 2共d兲兴. Therefore, along

D. Band edges at different depths

In most previous research on band edge calculation, the QD was assumed to be in an infinite substrate,31,32,36,37 which means the QD is surrounded by a thick substrate material without any influence from the external boundary or surface. However, QDs are more commonly found located near the interface or covered by a cap layer due to either fabrication procedures or, in some cases, by design to achieve novel device properties.40–43 In such applications, the effect of the free surface on band edges can be significant. Actually, Nishi et al.41 showed that the thick cap layer can produce a remarkable reduction in the photoluminescence 共PL兲 linewidth; Hugues et al.44 observed that a 5 nm Ga0.85In0.15As cap layer over the InAs QDs led to highly efficient emission of longer

073504-7

Pan et al.

J. Appl. Phys. 106, 073504 共2009兲

FIG. 5. 共Color online兲 Strain components 关共a兲 and 共c兲兴 and band edges 关共b兲 and 共d兲兴 in a pyramidal InAs/GaAs QD along the bottom center line of the QD 关共a兲 and 共b兲兴 in 共001兲 substrate and 关共c兲 and 共d兲兴 in 共111兲 substrate.

wavelength light with the latter being further attributed to the corresponding bandgap energy. To demonstrate the band edge differences in QDs located at different depths d in half-space substrates, we take the InAs cubic QD 关Fig. 1共a兲兴 as the example and use the exact method to carry out the numerical calculation. Shown in Figs. 9 and 10 are the HH, LH, and SO band edge variations along the bottom center line and along the z-axis for different embedding depths of the QD. In Fig. 10, the values ⫺2, 0, and 2 on the z-axis correspond, respectively, to the top, middle height, and bottom positions of the QD 关refer to Fig. 1共a兲 since the height of the QD is 4 nm兴. It is clear that when the buried QD is further beneath the free surface, from d = 4 nm to d = 24 nm 共distance d between the surface and middle height of cubic QD兲, the band edge curves gradually converge to the infinite-space solution with a decreasing trend. That is, the energy band edge variation becomes less and less as the QD moves away from the surface. This reasonable trend also indicates that when the depth of the QD reaches a critical value 共around 14 nm in this example兲, the substrate is effectively infinite.

E. Comparison with experimental results

We finally compare the energy bandgap from our calculations 共both exact and approximate k · p models兲 to previous experimental results41,44 in order to investigate the effect of the QD depth from the surface and to validate our analytical solutions. In our calculation, the InAs QDs are assumed to be in the InxGa1−xAs substrate with different depths 共or different cap layer thicknesses兲. Both PL measured and calculated bandgap energies are shown in Fig. 11. While we used the same QD size as those in Ref. 41, we chose the InAs QD with a large aspect ratio 共base= 20 nm; height= 5 nm兲 in order to compare the experimental results in Ref. 44 since no specific size information was available. Furthermore, a large aspect ratio is the general case for capped QDs,40–42,45 and it is also a dominant factor for band edge energy.31 We remark that since the PL measured result represents a volumetric average of the actual bandgap in the QD,4,46 it should therefore correspond to the accurate bandgap distribution predicted based on the exact k · p model.

073504-8

Pan et al.

J. Appl. Phys. 106, 073504 共2009兲

FIG. 6. 共Color online兲 Strain components 关共a兲 and 共c兲兴 and band edges 关共b兲 and 共d兲兴 in a pyramidal InAs/GaAs QD along the z-axis of the QD 关共a兲 and 共b兲兴 in 共001兲 substrate and 关共c兲 and 共d兲兴 in 共111兲 substrate.

As shown in Fig. 11, the bandgap energy from our calculation decreases with increasing depth of the QD 共or cap layer thickness兲, which is consistent with the redshift trend observed from experiments. In the limit, the energy level converges to the infinite-space substrate case. These results demonstrate the important effect of the surface on the energy band edge. Furthermore, compared to the experimental results, the bandgap energy based on the simplified approximate k · p model showed clearly a larger error than that based on the exact k · p model. We point out that the small differences in the energy between the experimental results and exact model could come from the small variation in the QD size and cap layer thickness, which would require precise measurements of these parameters in the future.

IV. CONCLUSIONS

In this article, we have studied the local band edge energies for zincblende InAs QDs in GaAs half-space substrates with full consideration of strains induced by the

lattice mismatch and influenced by the free surface. The strain fields are calculated by an accurate CM method based on the Eshelby inclusion model combined with the halfspace Green’s functions. By virtue of our CM method, a QD with any shape can be approximated by a number of flat triangles so that we can derive an analytical result for the strain fields. This method is particularly efficient when the QD surface is composed of facets. The strain-induced band edges in cubic and pyramidal InAs QDs 共embedded in a GaAs half-space substrate兲 are then calculated based on two 6 ⫻ 6 k · p models 共or approaches兲—one is inclusive of the detailed strain terms and the other is approximate 共the shear strain effect and the difference between the normal strains are neglected兲. Our numerical results indicate that the approximate model, which has been commonly adopted in literature,43,44 may lead to significant errors in the band edge energies. This is particularly true for points close to the boundary and/or corner of the QD where a relative error as large as 100% is observed. We have also calculated the strain-induced band edge in

073504-9

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

FIG. 7. 共Color online兲 Strain components 关共a兲 and 共c兲兴 and band edges 关共b兲 and 共d兲兴 in a pyramidal InAs/GaAs QD along the specified vertical line of the QD 关共a兲 and 共b兲兴 in 共001兲 substrate and 关共c兲 and 共d兲兴 in 共111兲 substrate.

the cubic QD embedded at different depths within the substrate. Our results show that these band edges are sensitive to the depth, indicating the importance of the free surface in band edge predictions. Our numerical results of band edge energies in QDs embedded in half-space substrates are further compared with existing experimental results. Such a comparison demonstrates that the analytical predictions based on the half-space substrate model with the exact k · p approach agree well with the experimental results while the approximate k · p approach shows an obvious and significant difference.

also like to thank the reviewer for his/her helpful comments and suggestions.

APPENDIX: STIFFNESS MATRICES OF GaAs AND InAs, AND BANDGAP PARAMETERS OF InAs 1. Stiffness matrix Cij in „109 N / m2…

The following are values for stiffness matrix Cij 共Ref. 27兲: 关CGaAs共001兲兴

ACKNOWLEDGMENTS

This work was partially supported by the National Natural Science Foundation of China Grant No. 10772106 共E.P.兲, by the Defense Threat Reduction Agency Joint Science and Technology Office 共DTRA-JSTO兲 under Grant No. W911NF-06-2-0038 共E.P. and P.W.C.兲, and by AFOSR Grant No. FA9550-06-1-0317 共Y.Z. and E.P.兲. The authors would

=

冤

118.8

53.8

53.8

0.0

0.0

0.0

118.8

53.8

0.0

0.0

0.0

118.8

0.0

0.0

0.0

59.4

0.0

0.0

59.4

0.0 59.4

冥

共A1兲

073504-10

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

FIG. 8. 共Color online兲 Relative error 共%兲 of the band edge calculations based on the approximate method as compared to the present exact method in an InAs/GaAs cubic QD embedded in GaAs 共001兲 and 共111兲 substrates: results along the bottom center line of the QD in 共a兲 and along the z-axis of the QD in 共b兲.

关CGaAs共111兲兴

=

冤 冤

145

45 145

36

0.0

12.7

36

0.0 − 12.7

0.0 0.0

154 0.0

0.0

0.0

41

0.0

− 12.7

41

0.0 50

冥

共A2兲

关CInAs共001兲兴

=

83.29 45.26 45.26

0.0

0.0

0.0

83.29 45.26

0.0

0.0

0.0

83.29

0.0

0.0

0.0

39.59

0.0

0.0

39.59

0.0 39.59

冥

FIG. 9. 共Color online兲 Band edges in a cubic QD embedded at different depths within the GaAs half-space substrate and in the infinite-space substrate along the bottom center line of the QD: 共a兲, 共b兲, and 共c兲 refer to the HH, LH, and SO bands, respectively.

共A3兲

2. Band parameters „in eV… for InAs

The following are band parameters for InAs 共Ref. 30兲: Eg0 = 0.413,

073504-11

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

FIG. 11. 共Color online兲 Comparison of bandgap energies between the experimental results and present calculations for InAs QDs within InxGa1−xAs substrates 共the k · p calculations are based on both the exact and approximate methods兲.

⌬SO = 0.38, ac = − 5.08, av = 1.00, b = − 1.80, d = − 3.60. 1

D. Bimberg, M. Grundmann, and N. N. Ledentsov, Quantum Dot Heterostructures 共Wiley, New York, 1999兲. J. Piprek, Semiconductor Optoelectronic Devices 共Academic, New York, 2003兲. 3 P. Y. Yu and M. Cardona, Fundamentals of Semiconductors 共Springer, New York, 2005兲. 4 H. Zhu, S. Feng, D. Jiang, Y. Deng, and H. Wang, Jpn. J. Appl. Phys., Part 1 38, 6264 共1999兲. 5 K. Kamath, H. Jiang, D. Klotzkin, J. Phillips, T. Sosnowski, T. Norris, J. Singh, and P. Bhattacharya, IEEE International Symposium on Compound Semiconductors, 1997 共unpublished兲, p. 525. 6 A. D. Andreev and E. P. O’Reilly, Phys. Rev. B 62, 15851 共2000兲. 7 V. Ranjan, G. Allan, C. Priester, and C. Delerue, Phys. Rev. B 68, 115305 共2003兲. 8 M. Grundmann, O. Stier, and D. Bimberg, Phys. Rev. B 52, 11969 共1995兲. 9 M. Califano and P. Harrison, J. Appl. Phys. 91, 389 共2002兲. 10 C. Pryor, J. Kim, L. W. Wang, A. J. Williamson, and A. Zunger, J. Appl. Phys. 83, 2548 共1998兲. 11 H. T. Johnson, L. B. Freund, C. D. Akyuz, and A. Zaslavsky, J. Appl. Phys. 84, 3714 共1998兲. 12 A. D. Andreev, J. R. Downes, D. A. Faux, and E. P. O’Reilly, J. Appl. Phys. 86, 297 共1999兲. 13 H. T. Johnson and L. B. Freund, Int. J. Solids Struct. 38, 1045 共2001兲. 14 A. J. Williamson, L. W. Wang, and A. Zunger, Phys. Rev. B 62, 12963 共2000兲. 15 M. Tadic, F. M. Peeters, K. L. Janssens, M. Korkusinski, and P. Hawrylak, J. Appl. Phys. 92, 5819 共2002兲. 16 L. C. Lew Yan Voon and L. R. Ram-Mohan, Phys. Rev. B 47, 15500 共1993兲. 17 E. Lidorikis, M. M. Sigalas, E. N. Economou, and C. M. Soukoulis, Phys. Rev. Lett. 81, 1405 共1998兲. 18 W. A. Harrison, Phys. Rev. B 77, 245103 共2008兲. 19 A. Valavanis, Z. Ikonic, and R. W. Kelsall, Phys. Rev. B 75, 205332 2

FIG. 10. 共Color online兲 Band edges in a cubic QD embedded at different depths within the GaAs half-space substrate and in the infinite-space substrate along the z-axis of the QD: 共a兲, 共b兲, and 共c兲 refer to the HH, LH, and SO bands, respectively.

073504-12

共2007兲. P. Piquini, A. Zunger, and R. Magri, Phys. Rev. B 77, 115314 共2008兲. 21 O. Stier, M. Grundmann, and D. Bimberg, Phys. Rev. B 59, 5688 共1999兲. 22 E. Pan, Y. Zhang, P. W. Chung, and M. Denda, Comput. Model. Eng. Sci. 841, 1 共2008兲. 23 T. C. T. Ting, Anisotropic Elasticity Theory and Applications 共Oxford Science, New York, 1996兲. 24 E. Pan, Proc. R. Soc. London, Ser. A 458, 181 共2002兲. 25 C. Y. Wang, M. Denda, and E. Pan, Int. J. Solids Struct. 43, 7593 共2006兲. 26 E. Pan and B. Yang, J. Appl. Phys. 90, 6190 共2001兲. 27 E. Pan, J. Appl. Phys. 91, 6379 共2002兲. 28 B. Yang and E. Pan, J. Appl. Phys. 92, 3084 共2002兲; E. Pan, F. Han, and J. D. Albrecht, ibid. 98, 013534 共2005兲. 29 S. W. Ellaway and D. A. Faux, J. Appl. Phys. 92, 3027 共2002兲. 30 I. Vurgaftman, J. R. Meyer, and L. R. Ram-Mohan, J. Appl. Phys. 89, 5815 共2001兲. 31 S. I. Rybchenko, G. Yeap, R. Gupta, I. E. Itskevich, and S. K. Haywood, J. Appl. Phys. 102, 013706 共2007兲. 32 A. Schliwa, M. Winkelnkemper, and D. Bimberg, Phys. Rev. B 76, 205324 共2007兲. 33 C. Y. Chao and S. L. Chuang, Phys. Rev. B 46, 4110 共1992兲. 20

J. Appl. Phys. 106, 073504 共2009兲

Pan et al.

J. M. Luttinger and W. Kohn, Phys. Rev. 97, 869 共1955兲. G. L. Bir and G. E. Pikus, Symmetry and Strain-Induced Effects in Semiconductors 共Wiley, New York, 1974兲. 36 C. Pryor, Phys. Rev. B 57, 7190 共1998兲. 37 C. Pryor, M.-E. Pistol, and L. Samuelson, Phys. Rev. B 56, 10404 共1997兲. 38 E. Pan, J. Appl. Phys. 91, 3785 共2002兲. 39 M. A. Cusack, P. R. Briddon, and M. Jaros, Phys. Rev. B 54, R2300 共1996兲. 40 K. Mukai and M. Sugawara, Appl. Phys. Lett. 74, 3963 共1999兲. 41 K. Nishi, H. Saito, S. Sugou, and J. S. Lee, Appl. Phys. Lett. 74, 1111 共1999兲. 42 Z. Gong, Z. D. Fang, Z. H. Miao, Z. C. Niu, and S. L. Feng, J. Cryst. Growth 274, 78 共2005兲. 43 M. Richter, B. Damilano, J. Y. Duboz, J. Massies, and A. D. Wieck, Appl. Phys. Lett. 88, 231902 共2006兲. 44 M. Hugues, M. Richter, B. Damilano, J. M. Chauveau, J. Y. Duboz, J. Massies, and A. D. Wieck, Phys. Status Solidi C 3, 3979 共2006兲. 45 J. Tatebayashi, M. Nishioka, and Y. Arakawa, Appl. Phys. Lett. 78, 3469 共2001兲. 46 Z. L. Miao, Y. W. Zhang, S. J. Chua, Y. H. Chye, P. Chen, and S. Tripathy, Appl. Phys. Lett. 86, 031914 共2005兲. 34 35